Ultrahigh Field Enhancement and Photoresponse in Atomically and fast photoresponse, and therefore...
Embed Size (px)
Transcript of Ultrahigh Field Enhancement and Photoresponse in Atomically and fast photoresponse, and therefore...
© 2015 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim 1wileyonlinelibrary.com
IC A TIO
Ultrahigh Field Enhancement and Photoresponse in Atomically Separated Arrays of Plasmonic Dimers
Debadrita Paria , Kallol Roy , Haobijam Johnson Singh , Shishir Kumar , Srinivasan Raghavan , Arindam Ghosh , and Ambarish Ghosh *
D. Paria, Dr. S. Kumar, Prof. S. Raghavan, Dr. A. Ghosh Centre for Nano Science and Engineering Indian Institute of Science Bangalore 560012 , India E-mail: email@example.com K. Roy, H. J. Singh, Prof. A. Ghosh, Dr. A. Ghosh Department of Physics Indian Institute of Science Bangalore 560012 , India Prof. S. Raghavan Materials Research Centre Indian Institute of Science Bangalore 560012 , India Dr. A. Ghosh Department of Electrical Communications Engineering Indian Institute of Science Bangalore 560012 , India
EM fi eld induced at their junction can get amplifi ed by several orders of magnitude, thereby facilitating two technologies of immense current interest. These so-called “hot spots” have facilitated the detection of single molecules through surface enhanced Raman spectroscopy (SERS), [ 3,4,6–8 ] which in turn inspired an entire fi eld of research devoted to the development of substrates containing metallic structures with nanosized gaps in between. Beside SERS applications, the enhanced EM fi eld at nanoparticle junctions can also be used to enhance the performance of various optoelectronic devices, such as those pertaining to photovoltaics [ 9 ] and high-speed wavelength-selec- tive photodetection.
In electrostatics, the electric fi eld between two oppositely charged plates varies inversely as the distance between them, which arises due to Coulomb interactions between the charges residing on the two plates. Similarly, the dependence of the EM fi eld enhancement [ 10 ] on the size of the gap ( d ) originates in the EM interactions between the localized plasmon modes of two neighboring nanoparticles (radius a ). In the simplest approximation, each particle can be approximated as an electric dipole pi
��� , whose strength is proportional to the net electric fi eld
(p aEi i ��� ���
= ) at its location, where a is the polarizabiltiy of the par- ticle at the wavelength of illumination. The contributions to the net electric fi eld for particle 1 come from the incident fi eld (E0
� �� ),
as well as the electric fi eld due to the dipole ( p2 ���
) of particle 2 at the location of particle 1, where the dominant term of E d2
3 � ��
∝ − , thus implying a strong distance dependence of the dipolar cou- pling. This approximation breaks down for d < a , beyond which higher order multipolar contributions needs to be taken into account, where numerical calculations can provide an accu- rate picture. Also important is the direction of propagation and state of polarization of the incident beam, and their relation to the interparticle axis. As an example, depicted schematically in Figure 1 a, we have considered linearly polarized monochro- matic light incident along the axis of the interparticle separa- tion for two silver nanospheres of radius a = 70 nm separated by a distance d . The calculated value of the squared enhance- ment (| E |/| E o |) 2 of the electric fi eld, shows concentration of the electric fi eld at the junction of the particles, which increases manifold as the distance d is reduced. The maximum value of the enhancement within the junction, given by (| E |/| E o |) 2 max , depended strongly on the illumination wavelength and the interparticle separation, as can be seen in Figure 1 b. The smallest d considered in these simulations corresponded to the thickness of single-layer graphene, which resulted in maximum value of(| E |/| E o |) 2 ≥ 10 6 in the wavelength regime 405 to 530 nm (approx), implying a system of plasmonic dimers with sub-nm separation can achieve the strongest EM fi eld enhancements.
The large concentration of electromagnetic (EM) fi elds near metal nanoparticles upon illumination of light is one of the defi ning concepts of light matter interactions at the nanoscale. [ 1,2 ] The strength of this so-called “near fi eld” can be very large at the junction of two metal nanoparticles, which has facilitated promising technologies, such as the detection of single molecules, [ 3,4 ] through a large enhancement of the Raman scattering signal. The degree of enhancement of the near fi eld increases rapidly as the particles are brought closer, thereby suggesting an atomically thin and uniform material, such as graphene, as the ideal spacer layer for maximum near fi eld enhancement. Here we combine oblique angle deposition (OAD) technique with standard graphene transfer protocols to fabricate two metal nanoparticle arrays separated precisely by a single layer of graphene (SLG). Upon illumination of light of appropriate wavelength, the optical near fi eld at the junction of the particles could be strongly enhanced which was refl ected in an order of magnitude increase of the Raman signal of the graphene monolayer. Most crucially, the enhanced near fi eld resulted in a dramatic increase of photoresponse in gra- phene [ 5 ] that allowed the realization of a new class of large-area color-selective plasmonic photodetectors. At room tempera- ture, the maximum responsivity of these devices approached 2 A W −1 , nearly two orders of magnitude greater than that of the of previous graphene-based plasmonic devices, which sig- nify the tremendous promise of this novel method of inte- grating plasmonics with graphene and other atomically thin materials.
When two nanoparticles made of noble metals under appro- priate illumination are placed within few nm of each other, the
Adv. Mater. 2015, DOI: 10.1002/adma.201404312
2 wileyonlinelibrary.com © 2015 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim
IC A TI
The distance dependence of (| E |/| E o |) 2 max for three illumination wavelengths is shown in Figure 1 c.
The engineering challenges to develop such a system are primarily related to the smallest gap that can be reliably and reproducibly obtained with the chosen method of fabrication, with a possible emphasis towards the development of large area substrates using scalable techniques. Commonly used systems, such as aggregates of metal colloids, suffer from the random- ness of the gap size and therefore the EM fi eld enhancement, whereas the typical resolution [ 11 ] achievable with electron beam lithography being greater than 5 nm, renders standard litho- graphic approaches mostly ineffective. Among various wafer scale methods, the array of metallic nanopyramids obtained with nanosphere lithography [ 12 ] is common, although it suffers from the nonuniformity of the gap sizes below few nm. This is also true for recently reported [ 13 ] self-assembled pair of gold nanorods whose separations varied between 0.5 and 2 nm. Alter- nate approaches towards fabricating uniform and reproducible nm sized gaps have relied on using a thin spacer material, such as polyelectrolyte [ 14 ] coating (thickness > 3 nm) or SLG [ 15 ] (spacing 0.34 nm) separating a collection of gold colloids from a thin fi lm, also made of gold. One shortcoming of this method is related to the conductivity of the underlying metal fi lm, which makes this method incompatible with applications aiming towards improving the photodetection effi ciency of the thin spacer material. The solution that presents itself is therefore
not to use a gold fi lm, but rather place a spacer material between a pair [ 16–18 ] of metal nanoparticles. For realistic appli- cations requiring large area devices, an attractive possibility would be to use two arrays of plasmonic nanoparticles sepa- rated by a suitable spacer material, which by virtue of its large near fi eld focusing, can be used as a sensitive SERS substrate, and as a photoresponsive device as well. As we demonstrate in this paper, an almost ideal solution can be achieved with a SLG acting as a spacer between two arrays of silver nanoparticles, giving rise to extremely large and localized EM fi elds, resulting in a 100-fold enhancement of the SLG photoresponse.
Three properties of graphene make it an ideal candidate as a spacer material: (i) graphene can be used as a standard for Raman [ 19–22 ] measurements, since its Raman scattering is highly reproducible and well understood. Additionally, it is pos- sible to functionalize graphene with various chemicals, which in conjunction with the highly enhanced near fi eld, allows graphene to be an ideal substrate for SERS measurements. (ii) In spite of its low absorption, graphene shows broadband and fast photoresponse, and therefore promising as a mate- rial for photodetection. (iii) Most importantly, it is one of the thinnest materials available, with thickness precisely that of an atom (0.34 nm), thereby allowing a very large enhancement of the EM fi eld at the junction of the nanoparticles, as shown in Figure 1 c. An important question that arises is whether this is the highest fi eld enhancement one could achieve, or
Adv. Mater. 2015, DOI: 10.1002/adma.201404312